#------------------------------------------------------------------------------
#$Date: 2016-03-23 23:57:12 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179519 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/16/4341664.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341664
loop_
_publ_author_name
'Treadwell, LaRico J'
'Watkins-Curry, Pilanda'
'McAlpin, Jacob D.'
'Rebar, Drew J.'
'Hebert, Jessica K.'
'DiTusa, John F.'
'Chan, Julia Y.'
_publ_section_title
;
 Investigation of Mn, Fe, and Ni Incorporation in CeCo2Al8.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              963
_journal_page_last               968
_journal_paper_doi               10.1021/ic502356t
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'Al8 Ce Co1.33 Fe0.67'
_chemical_formula_sum            'Al8 Ce Co1.33 Fe0.67'
_chemical_formula_weight         470.74
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           55
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2014-10-27 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.4820(5)
_cell_length_b                   14.401(3)
_cell_length_c                   4.029(3)
_cell_measurement_temperature    293(2)
_cell_volume                     724.2(6)
_computing_cell_refinement       'Denzo and Scalepack (Otwinski & Minor 1997)'
_computing_data_collection       'Collect (Nonius 1999)'
_computing_data_reduction        'Denzo and Scalepack (Otwinski & Minor 1997)'
_computing_molecular_graphics    'Crystal Maker'
_computing_publication_material  Publcif
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Nonius Kappa CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0263
_diffrn_reflns_av_sigmaI/netI    0.0325
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            2143
_diffrn_reflns_theta_full        30.99
_diffrn_reflns_theta_max         30.99
_diffrn_reflns_theta_min         3.26
_exptl_absorpt_coefficient_mu    11.285
_exptl_absorpt_correction_T_max  0.713
_exptl_absorpt_correction_T_min  0.673
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL scalepack (Otwinski & Minor, 1997)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.317
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Fragment
_exptl_crystal_F_000             860
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.442
_refine_diff_density_min         -2.187
_refine_diff_density_rms         0.295
_refine_ls_extinction_coef       0.0299(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.973
_refine_ls_matrix_type           full
_refine_ls_number_parameters     74
_refine_ls_number_reflns         1299
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      0.973
_refine_ls_R_factor_all          0.0374
_refine_ls_R_factor_gt           0.0288
_refine_ls_shift/su_max          0.008
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0388P)²+3.0837P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0678
_refine_ls_wR_factor_ref         0.0725
_reflns_number_gt                1092
_reflns_number_total             1299
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic502356t_si_004.cif
_cod_data_source_block           shelx
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4341656--4341665.cif.
;
_cod_original_cell_volume        724.2(5)
_cod_original_sg_symbol_H-M      Pbam
_cod_database_code               4341664
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'-x-1/2, y-1/2, z'
'x-1/2, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ce1 Ce 0.34100(2) 0.31860(2) 0.0000 0.01089(12) Uani 1 2 d S
Co2 Co 0.15081(5) 0.09686(5) 0.0000 0.0081(3) Uani 0.56(6) 2 d SP
Fe2 Fe 0.15081(5) 0.09686(5) 0.0000 0.0081(3) Uani 0.44(7) 2 d SP
Co1 Co 0.03429(6) 0.40652(5) 0.0000 0.0094(2) Uani 0.77(6) 2 d SP
Fe1 Fe 0.03429(6) 0.40652(5) 0.0000 0.0094(2) Uani 0.21(7) 2 d SP
Al8 Al 0.0000 0.5000 0.5000 0.0104(4) Uani 1 4 d S
Al9 Al 0.0000 0.0000 0.0000 0.0116(4) Uani 1 4 d S
Al2 Al 0.15973(12) 0.37907(12) 0.5000 0.0102(3) Uani 1 2 d S
Al5 Al 0.45244(13) 0.17980(11) 0.5000 0.0106(3) Uani 1 2 d S
Al3 Al 0.23576(13) 0.17268(11) 0.5000 0.0104(3) Uani 1 2 d S
Al4 Al 0.33143(13) 0.49209(11) 0.5000 0.0103(3) Uani 1 2 d S
Al1 Al 0.02565(13) 0.13191(11) 0.5000 0.0102(3) Uani 1 2 d S
Al7 Al 0.33857(12) 0.04450(12) 0.0000 0.0120(3) Uani 1 2 d S
Al6 Al 0.09556(12) 0.25325(10) 0.0000 0.0105(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al1 Ce1 Al1 79.72(5) 3_556 3
Al1 Ce1 Al2 93.10(4) 3_556 .
Al1 Ce1 Al2 150.85(5) 3 .
Al1 Ce1 Al2 150.85(5) 3_556 1_554
Al1 Ce1 Al2 93.10(4) 3 1_554
Al2 Ce1 Al2 79.45(5) . 1_554
Al1 Ce1 Al5 53.99(4) 3_556 .
Al1 Ce1 Al5 103.25(4) 3 .
Al2 Ce1 Al5 94.78(4) . .
Al2 Ce1 Al5 153.90(4) 1_554 .
Al1 Ce1 Al5 103.25(4) 3_556 1_554
Al1 Ce1 Al5 53.99(4) 3 1_554
Al2 Ce1 Al5 153.90(4) . 1_554
Al2 Ce1 Al5 94.78(4) 1_554 1_554
Al5 Ce1 Al5 79.20(5) . 1_554
Al1 Ce1 Al3 148.77(4) 3_556 1_554
Al1 Ce1 Al3 92.67(4) 3 1_554
Al2 Ce1 Al3 106.84(4) . 1_554
Al2 Ce1 Al3 58.90(4) 1_554 1_554
Al5 Ce1 Al3 99.61(4) . 1_554
Al5 Ce1 Al3 50.42(4) 1_554 1_554
Al1 Ce1 Al3 92.67(4) 3_556 .
Al1 Ce1 Al3 148.77(4) 3 .
Al2 Ce1 Al3 58.90(4) . .
Al2 Ce1 Al3 106.84(4) 1_554 .
Al5 Ce1 Al3 50.42(4) . .
Al5 Ce1 Al3 99.61(4) 1_554 .
Al3 Ce1 Al3 78.22(5) 1_554 .
Al1 Ce1 Al6 140.14(3) 3_556 .
Al1 Ce1 Al6 140.14(3) 3 .
Al2 Ce1 Al6 52.77(3) . .
Al2 Ce1 Al6 52.77(3) 1_554 .
Al5 Ce1 Al6 103.59(4) . .
Al5 Ce1 Al6 103.59(4) 1_554 .
Al3 Ce1 Al6 54.10(3) 1_554 .
Al3 Ce1 Al6 54.10(3) . .
Al1 Ce1 Al4 104.65(4) 3_556 1_554
Al1 Ce1 Al4 56.55(4) 3 1_554
Al2 Ce1 Al4 99.17(4) . 1_554
Al2 Ce1 Al4 50.02(4) 1_554 1_554
Al5 Ce1 Al4 155.25(4) . 1_554
Al5 Ce1 Al4 96.23(4) 1_554 1_554
Al3 Ce1 Al4 95.79(4) 1_554 1_554
Al3 Ce1 Al4 153.16(4) . 1_554
Al6 Ce1 Al4 101.12(4) . 1_554
Al1 Ce1 Al4 56.55(4) 3_556 .
Al1 Ce1 Al4 104.65(4) 3 .
Al2 Ce1 Al4 50.02(4) . .
Al2 Ce1 Al4 99.17(4) 1_554 .
Al5 Ce1 Al4 96.23(4) . .
Al5 Ce1 Al4 155.25(4) 1_554 .
Al3 Ce1 Al4 153.16(4) 1_554 .
Al3 Ce1 Al4 95.79(4) . .
Al6 Ce1 Al4 101.12(4) . .
Al4 Ce1 Al4 77.70(5) 1_554 .
Al1 Ce1 Al9 51.38(3) 3_556 3
Al1 Ce1 Al9 51.38(3) 3 3
Al2 Ce1 Al9 102.37(3) . 3
Al2 Ce1 Al9 102.37(3) 1_554 3
Al5 Ce1 Al9 103.73(3) . 3
Al5 Ce1 Al9 103.73(3) 1_554 3
Al3 Ce1 Al9 140.60(2) 1_554 3
Al3 Ce1 Al9 140.60(3) . 3
Al6 Ce1 Al9 144.30(3) . 3
Al4 Ce1 Al9 53.35(3) 1_554 3
Al4 Ce1 Al9 53.35(3) . 3
Al9 Co2 Al6 109.51(5) . .
Al9 Co2 Al7 125.62(5) . .
Al6 Co2 Al7 124.86(6) . .
Al9 Co2 Al3 126.50(4) . .
Al6 Co2 Al3 73.11(4) . .
Al7 Co2 Al3 74.49(5) . .
Al9 Co2 Al3 126.50(4) . 1_554
Al6 Co2 Al3 73.11(4) . 1_554
Al7 Co2 Al3 74.49(5) . 1_554
Al3 Co2 Al3 105.86(7) . 1_554
Al9 Co2 Al4 73.44(4) . 7_654
Al6 Co2 Al4 126.63(4) . 7_654
Al7 Co2 Al4 74.55(5) . 7_654
Al3 Co2 Al4 149.04(6) . 7_654
Al3 Co2 Al4 65.50(5) 1_554 7_654
Al9 Co2 Al4 73.44(4) . 7_655
Al6 Co2 Al4 126.63(4) . 7_655
Al7 Co2 Al4 74.55(5) . 7_655
Al3 Co2 Al4 65.50(5) . 7_655
Al3 Co2 Al4 149.04(6) 1_554 7_655
Al4 Co2 Al4 105.74(7) 7_654 7_655
Al9 Co2 Al1 68.45(4) . 1_554
Al6 Co2 Al1 68.79(4) . 1_554
Al7 Co2 Al1 129.18(3) . 1_554
Al3 Co2 Al1 141.91(6) . 1_554
Al3 Co2 Al1 63.25(5) 1_554 1_554
Al4 Co2 Al1 63.30(5) 7_654 1_554
Al4 Co2 Al1 141.88(6) 7_655 1_554
Al9 Co2 Al1 68.45(4) . .
Al6 Co2 Al1 68.79(4) . .
Al7 Co2 Al1 129.18(3) . .
Al3 Co2 Al1 63.25(5) . .
Al3 Co2 Al1 141.90(6) 1_554 .
Al4 Co2 Al1 141.88(6) 7_654 .
Al4 Co2 Al1 63.30(5) 7_655 .
Al1 Co2 Al1 101.64(7) 1_554 .
Al6 Co1 Al8 125.03(2) . .
Al6 Co1 Al8 125.03(2) . 1_554
Al8 Co1 Al8 109.92(4) . 1_554
Al6 Co1 Al7 122.28(6) . 7_665
Al8 Co1 Al7 71.40(3) . 7_665
Al8 Co1 Al7 71.40(3) 1_554 7_665
Al6 Co1 Al7 125.22(6) . 3_455
Al8 Co1 Al7 71.40(3) . 3_455
Al8 Co1 Al7 71.40(3) 1_554 3_455
Al7 Co1 Al7 112.50(5) 7_665 3_455
Al6 Co1 Al5 70.99(4) . 3_455
Al8 Co1 Al5 146.58(5) . 3_455
Al8 Co1 Al5 63.59(4) 1_554 3_455
Al7 Co1 Al5 128.61(3) 7_665 3_455
Al7 Co1 Al5 75.70(4) 3_455 3_455
Al6 Co1 Al5 70.99(4) . 3_456
Al8 Co1 Al5 63.59(4) . 3_456
Al8 Co1 Al5 146.58(5) 1_554 3_456
Al7 Co1 Al5 128.61(3) 7_665 3_456
Al7 Co1 Al5 75.70(5) 3_455 3_456
Al5 Co1 Al5 102.77(7) 3_455 3_456
Al6 Co1 Al2 69.93(5) . 1_554
Al8 Co1 Al2 145.90(5) . 1_554
Al8 Co1 Al2 63.28(4) 1_554 1_554
Al7 Co1 Al2 75.00(5) 7_665 1_554
Al7 Co1 Al2 128.69(3) 3_455 1_554
Al5 Co1 Al2 63.69(5) 3_455 1_554
Al5 Co1 Al2 140.91(6) 3_456 1_554
Al6 Co1 Al2 69.93(5) . .
Al8 Co1 Al2 63.28(4) . .
Al8 Co1 Al2 145.90(5) 1_554 .
Al7 Co1 Al2 75.00(5) 7_665 .
Al7 Co1 Al2 128.69(3) 3_455 .
Al5 Co1 Al2 140.91(6) 3_455 .
Al5 Co1 Al2 63.69(5) 3_456 .
Al2 Co1 Al2 102.57(7) 1_554 .
Al6 Co1 Co1 178.52(6) . 5_565
Al8 Co1 Co1 54.96(2) . 5_565
Al8 Co1 Co1 54.96(2) 1_554 5_565
Al7 Co1 Co1 56.25(4) 7_665 5_565
Al7 Co1 Co1 56.26(5) 3_455 5_565
Al5 Co1 Co1 109.84(4) 3_455 5_565
Al5 Co1 Co1 109.84(4) 3_456 5_565
Al2 Co1 Co1 109.25(4) 1_554 5_565
Al2 Co1 Co1 109.25(4) . 5_565
Al6 Co1 Fe1 178.52(6) . 5_565
Al8 Co1 Fe1 54.96(2) . 5_565
Al8 Co1 Fe1 54.96(2) 1_554 5_565
Al7 Co1 Fe1 56.25(4) 7_665 5_565
Al7 Co1 Fe1 56.26(5) 3_455 5_565
Al5 Co1 Fe1 109.84(4) 3_455 5_565
Al5 Co1 Fe1 109.84(4) 3_456 5_565
Al2 Co1 Fe1 109.25(4) 1_554 5_565
Al2 Co1 Fe1 109.25(4) . 5_565
Co1 Co1 Fe1 0.00(3) 5_565 5_565
Fe1 Al8 Co1 0.00(3) 5_566 5_566
Fe1 Al8 Fe1 109.92(4) 5_566 5_565
Co1 Al8 Fe1 109.92(4) 5_566 5_565
Fe1 Al8 Fe1 70.08(4) 5_566 1_556
Co1 Al8 Fe1 70.08(4) 5_566 1_556
Fe1 Al8 Fe1 180.00(3) 5_565 1_556
Fe1 Al8 Co1 70.08(4) 5_566 1_556
Co1 Al8 Co1 70.08(4) 5_566 1_556
Fe1 Al8 Co1 180.00(3) 5_565 1_556
Fe1 Al8 Co1 0.00(4) 1_556 1_556
Fe1 Al8 Co1 109.92(4) 5_566 5_565
Co1 Al8 Co1 109.92(4) 5_566 5_565
Fe1 Al8 Co1 0.00(4) 5_565 5_565
Fe1 Al8 Co1 180.0 1_556 5_565
Co1 Al8 Co1 180.0 1_556 5_565
Fe1 Al8 Co1 180.0 5_566 .
Co1 Al8 Co1 180.0 5_566 .
Fe1 Al8 Co1 70.08(4) 5_565 .
Fe1 Al8 Co1 109.92(4) 1_556 .
Co1 Al8 Co1 109.92(4) 1_556 .
Co1 Al8 Co1 70.08(4) 5_565 .
Fe1 Al8 Al2 119.40(2) 5_566 .
Co1 Al8 Al2 119.40(2) 5_566 .
Fe1 Al8 Al2 119.40(2) 5_565 .
Fe1 Al8 Al2 60.60(2) 1_556 .
Co1 Al8 Al2 60.60(2) 1_556 .
Co1 Al8 Al2 119.40(2) 5_565 .
Co1 Al8 Al2 60.60(2) . .
Fe1 Al8 Al2 60.60(2) 5_566 5_566
Co1 Al8 Al2 60.60(2) 5_566 5_566
Fe1 Al8 Al2 60.60(2) 5_565 5_566
Fe1 Al8 Al2 119.40(2) 1_556 5_566
Co1 Al8 Al2 119.40(2) 1_556 5_566
Co1 Al8 Al2 60.60(2) 5_565 5_566
Co1 Al8 Al2 119.40(2) . 5_566
Al2 Al8 Al2 180.0 . 5_566
Fe1 Al8 Al5 60.37(2) 5_566 7_665
Co1 Al8 Al5 60.37(2) 5_566 7_665
Fe1 Al8 Al5 60.37(2) 5_565 7_665
Fe1 Al8 Al5 119.63(2) 1_556 7_665
Co1 Al8 Al5 119.63(2) 1_556 7_665
Co1 Al8 Al5 60.37(2) 5_565 7_665
Co1 Al8 Al5 119.63(2) . 7_665
Al2 Al8 Al5 118.23(5) . 7_665
Al2 Al8 Al5 61.77(5) 5_566 7_665
Fe1 Al8 Al5 119.63(2) 5_566 3_456
Co1 Al8 Al5 119.63(2) 5_566 3_456
Fe1 Al8 Al5 119.63(2) 5_565 3_456
Fe1 Al8 Al5 60.37(2) 1_556 3_456
Co1 Al8 Al5 60.37(2) 1_556 3_456
Co1 Al8 Al5 119.63(2) 5_565 3_456
Co1 Al8 Al5 60.37(2) . 3_456
Al2 Al8 Al5 61.77(5) . 3_456
Al2 Al8 Al5 118.23(5) 5_566 3_456
Al5 Al8 Al5 180.0 7_665 3_456
Co2 Al9 Fe2 180.0 . 5
Co2 Al9 Co2 180.0 . 5
Fe2 Al9 Co2 0.00(3) 5 5
Co2 Al9 Al1 119.87(3) . 5
Fe2 Al9 Al1 60.13(3) 5 5
Co2 Al9 Al1 60.13(3) 5 5
Co2 Al9 Al1 119.87(3) . 5_556
Fe2 Al9 Al1 60.13(3) 5 5_556
Co2 Al9 Al1 60.13(3) 5 5_556
Al1 Al9 Al1 92.56(6) 5 5_556
Co2 Al9 Al1 60.13(3) . 1_554
Fe2 Al9 Al1 119.87(3) 5 1_554
Co2 Al9 Al1 119.87(3) 5 1_554
Al1 Al9 Al1 87.44(6) 5 1_554
Al1 Al9 Al1 180.00(8) 5_556 1_554
Co2 Al9 Al1 60.13(3) . .
Fe2 Al9 Al1 119.87(3) 5 .
Co2 Al9 Al1 119.87(3) 5 .
Al1 Al9 Al1 180.0 5 .
Al1 Al9 Al1 87.44(6) 5_556 .
Al1 Al9 Al1 92.56(6) 1_554 .
Co2 Al9 Al4 123.82(3) . 3_455
Fe2 Al9 Al4 56.18(3) 5 3_455
Co2 Al9 Al4 56.18(3) 5 3_455
Al1 Al9 Al4 56.24(5) 5 3_455
Al1 Al9 Al4 116.31(5) 5_556 3_455
Al1 Al9 Al4 63.69(5) 1_554 3_455
Al1 Al9 Al4 123.76(5) . 3_455
Co2 Al9 Al4 56.18(3) . 7_655
Fe2 Al9 Al4 123.82(3) 5 7_655
Co2 Al9 Al4 123.82(3) 5 7_655
Al1 Al9 Al4 123.76(5) 5 7_655
Al1 Al9 Al4 63.69(5) 5_556 7_655
Al1 Al9 Al4 116.31(5) 1_554 7_655
Al1 Al9 Al4 56.24(5) . 7_655
Al4 Al9 Al4 180.00(7) 3_455 7_655
Co2 Al9 Al4 123.82(3) . 3_456
Fe2 Al9 Al4 56.18(3) 5 3_456
Co2 Al9 Al4 56.18(3) 5 3_456
Al1 Al9 Al4 116.31(5) 5 3_456
Al1 Al9 Al4 56.24(5) 5_556 3_456
Al1 Al9 Al4 123.76(5) 1_554 3_456
Al1 Al9 Al4 63.70(5) . 3_456
Al4 Al9 Al4 87.42(6) 3_455 3_456
Al4 Al9 Al4 92.58(6) 7_655 3_456
Co2 Al9 Al4 56.18(3) . 7_654
Fe2 Al9 Al4 123.82(3) 5 7_654
Co2 Al9 Al4 123.82(3) 5 7_654
Al1 Al9 Al4 63.69(5) 5 7_654
Al1 Al9 Al4 123.76(5) 5_556 7_654
Al1 Al9 Al4 56.24(5) 1_554 7_654
Al1 Al9 Al4 116.30(5) . 7_654
Al4 Al9 Al4 92.58(6) 3_455 7_654
Al4 Al9 Al4 87.42(6) 7_655 7_654
Al4 Al9 Al4 180.00(4) 3_456 7_654
Co1 Al2 Fe1 102.57(7) . 1_556
Co1 Al2 Co1 102.57(7) . 1_556
Fe1 Al2 Co1 0.00(4) 1_556 1_556
Co1 Al2 Al8 56.12(4) . .
Fe1 Al2 Al8 56.12(4) 1_556 .
Co1 Al2 Al8 56.12(4) 1_556 .
Co1 Al2 Al4 112.98(5) . .
Fe1 Al2 Al4 112.98(5) 1_556 .
Co1 Al2 Al4 112.98(5) 1_556 .
Al8 Al2 Al4 101.65(7) . .
Co1 Al2 Al5 58.09(4) . 3_456
Fe1 Al2 Al5 58.09(4) 1_556 3_456
Co1 Al2 Al5 58.09(4) 1_556 3_456
Al8 Al2 Al5 59.28(5) . 3_456
Al4 Al2 Al5 160.93(8) . 3_456
Co1 Al2 Al6 50.94(4) . .
Fe1 Al2 Al6 118.85(7) 1_556 .
Co1 Al2 Al6 118.85(7) 1_556 .
Al8 Al2 Al6 102.03(5) . .
Al4 Al2 Al6 127.85(5) . .
Al5 Al2 Al6 62.03(5) 3_456 .
Co1 Al2 Al6 118.85(7) . 1_556
Fe1 Al2 Al6 50.95(4) 1_556 1_556
Co1 Al2 Al6 50.95(4) 1_556 1_556
Al8 Al2 Al6 102.03(5) . 1_556
Al4 Al2 Al6 127.85(5) . 1_556
Al5 Al2 Al6 62.03(5) 3_456 1_556
Al6 Al2 Al6 90.96(7) . 1_556
Co1 Al2 Ce1 167.49(5) . 1_556
Fe1 Al2 Ce1 88.79(4) 1_556 1_556
Co1 Al2 Ce1 88.79(4) 1_556 1_556
Al8 Al2 Ce1 136.25(4) . 1_556
Al4 Al2 Ce1 66.14(4) . 1_556
Al5 Al2 Ce1 126.59(5) 3_456 1_556
Al6 Al2 Ce1 118.82(6) . 1_556
Al6 Al2 Ce1 64.57(4) 1_556 1_556
Co1 Al2 Ce1 88.79(4) . .
Fe1 Al2 Ce1 167.49(5) 1_556 .
Co1 Al2 Ce1 167.49(5) 1_556 .
Al8 Al2 Ce1 136.25(4) . .
Al4 Al2 Ce1 66.14(4) . .
Al5 Al2 Ce1 126.59(5) 3_456 .
Al6 Al2 Ce1 64.57(4) . .
Al6 Al2 Ce1 118.82(6) 1_556 .
Ce1 Al2 Ce1 79.45(5) 1_556 .
Fe1 Al5 Co1 0.00(3) 3 3
Fe1 Al5 Fe1 102.77(7) 3 3_556
Co1 Al5 Fe1 102.77(7) 3 3_556
Fe1 Al5 Co1 102.77(7) 3 3_556
Co1 Al5 Co1 102.77(7) 3 3_556
Fe1 Al5 Co1 0.00(3) 3_556 3_556
Fe1 Al5 Al8 56.05(4) 3 3_556
Co1 Al5 Al8 56.05(4) 3 3_556
Fe1 Al5 Al8 56.05(4) 3_556 3_556
Co1 Al5 Al8 56.05(4) 3_556 3_556
Fe1 Al5 Al3 112.19(5) 3 .
Co1 Al5 Al3 112.19(5) 3 .
Fe1 Al5 Al3 112.19(5) 3_556 .
Co1 Al5 Al3 112.19(5) 3_556 .
Al8 Al5 Al3 100.74(6) 3_556 .
Fe1 Al5 Al2 58.22(4) 3 3_556
Co1 Al5 Al2 58.22(4) 3 3_556
Fe1 Al5 Al2 58.22(4) 3_556 3_556
Co1 Al5 Al2 58.22(4) 3_556 3_556
Al8 Al5 Al2 58.95(5) 3_556 3_556
Al3 Al5 Al2 159.69(8) . 3_556
Fe1 Al5 Al6 117.74(7) 3 3_556
Co1 Al5 Al6 117.74(7) 3 3_556
Fe1 Al5 Al6 50.55(4) 3_556 3_556
Co1 Al5 Al6 50.55(4) 3_556 3_556
Al8 Al5 Al6 100.89(5) 3_556 3_556
Al3 Al5 Al6 129.57(5) . 3_556
Al2 Al5 Al6 60.75(5) 3_556 3_556
Fe1 Al5 Al6 50.55(4) 3 3
Co1 Al5 Al6 50.55(4) 3 3
Fe1 Al5 Al6 117.74(7) 3_556 3
Co1 Al5 Al6 117.74(7) 3_556 3
Al8 Al5 Al6 100.89(5) 3_556 3
Al3 Al5 Al6 129.57(5) . 3
Al2 Al5 Al6 60.75(5) 3_556 3
Al6 Al5 Al6 89.56(7) 3_556 3
Fe1 Al5 Al1 109.29(5) 3 3_556
Co1 Al5 Al1 109.29(5) 3 3_556
Fe1 Al5 Al1 109.29(5) 3_556 3_556
Co1 Al5 Al1 109.29(5) 3_556 3_556
Al8 Al5 Al1 148.46(7) 3_556 3_556
Al3 Al5 Al1 110.80(7) . 3_556
Al2 Al5 Al1 89.52(7) 3_556 3_556
Al6 Al5 Al1 58.74(5) 3_556 3_556
Al6 Al5 Al1 58.74(5) 3 3_556
Fe1 Al5 Ce1 88.93(4) 3 .
Co1 Al5 Ce1 88.93(4) 3 .
Fe1 Al5 Ce1 167.79(5) 3_556 .
Co1 Al5 Ce1 167.79(5) 3_556 .
Al8 Al5 Ce1 135.63(3) 3_556 .
Al3 Al5 Ce1 65.43(4) . .
Al2 Al5 Ce1 127.96(4) 3_556 .
Al6 Al5 Ce1 120.71(6) 3_556 .
Al6 Al5 Ce1 67.22(4) 3 .
Al1 Al5 Ce1 62.69(4) 3_556 .
Fe1 Al5 Ce1 167.79(5) 3 1_556
Co1 Al5 Ce1 167.79(5) 3 1_556
Fe1 Al5 Ce1 88.93(4) 3_556 1_556
Co1 Al5 Ce1 88.93(4) 3_556 1_556
Al8 Al5 Ce1 135.63(3) 3_556 1_556
Al3 Al5 Ce1 65.43(4) . 1_556
Al2 Al5 Ce1 127.96(4) 3_556 1_556
Al6 Al5 Ce1 67.22(4) 3_556 1_556
Al6 Al5 Ce1 120.71(6) 3 1_556
Al1 Al5 Ce1 62.69(4) 3_556 1_556
Ce1 Al5 Ce1 79.20(5) . 1_556
Fe2 Al3 Co2 0.00(4) 1_556 1_556
Fe2 Al3 Co2 105.86(7) 1_556 .
Co2 Al3 Co2 105.86(7) 1_556 .
Fe2 Al3 Al1 59.72(4) 1_556 .
Co2 Al3 Al1 59.72(4) 1_556 .
Co2 Al3 Al1 59.72(4) . .
Fe2 Al3 Al5 115.85(5) 1_556 .
Co2 Al3 Al5 115.85(5) 1_556 .
Co2 Al3 Al5 115.85(5) . .
Al1 Al3 Al5 169.56(8) . .
Fe2 Al3 Al4 57.29(4) 1_556 7_655
Co2 Al3 Al4 57.29(4) 1_556 7_655
Co2 Al3 Al4 57.29(4) . 7_655
Al1 Al3 Al4 59.51(6) . 7_655
Al5 Al3 Al4 110.05(7) . 7_655
Fe2 Al3 Al6 50.76(4) 1_556 1_556
Co2 Al3 Al6 50.76(4) 1_556 1_556
Co2 Al3 Al6 118.18(7) . 1_556
Al1 Al3 Al6 60.01(5) . 1_556
Al5 Al3 Al6 125.86(5) . 1_556
Al4 Al3 Al6 101.24(6) 7_655 1_556
Fe2 Al3 Al6 118.18(7) 1_556 .
Co2 Al3 Al6 118.18(7) 1_556 .
Co2 Al3 Al6 50.76(4) . .
Al1 Al3 Al6 60.01(5) . .
Al5 Al3 Al6 125.86(5) . .
Al4 Al3 Al6 101.24(6) 7_655 .
Al6 Al3 Al6 87.63(7) 1_556 .
Fe2 Al3 Ce1 163.85(5) 1_556 .
Co2 Al3 Ce1 163.85(5) 1_556 .
Co2 Al3 Ce1 87.36(4) . .
Al1 Al3 Ce1 123.03(5) . .
Al5 Al3 Ce1 64.15(4) . .
Al4 Al3 Ce1 138.81(3) 7_655 .
Al6 Al3 Ce1 114.94(6) 1_556 .
Al6 Al3 Ce1 63.15(4) . .
Fe2 Al3 Ce1 87.36(4) 1_556 1_556
Co2 Al3 Ce1 87.36(4) 1_556 1_556
Co2 Al3 Ce1 163.85(5) . 1_556
Al1 Al3 Ce1 123.03(5) . 1_556
Al5 Al3 Ce1 64.16(4) . 1_556
Al4 Al3 Ce1 138.81(3) 7_655 1_556
Al6 Al3 Ce1 63.14(4) 1_556 1_556
Al6 Al3 Ce1 114.94(6) . 1_556
Ce1 Al3 Ce1 78.21(5) . 1_556
Fe2 Al4 Co2 0.00(3) 7_666 7_666
Fe2 Al4 Fe2 105.75(7) 7_666 7_665
Co2 Al4 Fe2 105.75(7) 7_666 7_665
Fe2 Al4 Co2 105.75(7) 7_666 7_665
Co2 Al4 Co2 105.75(7) 7_666 7_665
Fe2 Al4 Co2 0.00(4) 7_665 7_665
Fe2 Al4 Al1 59.66(4) 7_666 7_665
Co2 Al4 Al1 59.66(4) 7_666 7_665
Fe2 Al4 Al1 59.66(4) 7_665 7_665
Co2 Al4 Al1 59.66(4) 7_665 7_665
Fe2 Al4 Al2 115.53(5) 7_666 .
Co2 Al4 Al2 115.53(5) 7_666 .
Fe2 Al4 Al2 115.53(5) 7_665 .
Co2 Al4 Al2 115.53(5) 7_665 .
Al1 Al4 Al2 168.75(8) 7_665 .
Fe2 Al4 Al3 57.22(4) 7_666 7_665
Co2 Al4 Al3 57.22(4) 7_666 7_665
Fe2 Al4 Al3 57.22(4) 7_665 7_665
Co2 Al4 Al3 57.22(4) 7_665 7_665
Al1 Al4 Al3 59.41(6) 7_665 7_665
Al2 Al4 Al3 109.34(7) . 7_665
Fe2 Al4 Al9 50.39(3) 7_666 3_556
Co2 Al4 Al9 50.39(3) 7_666 3_556
Fe2 Al4 Al9 117.67(6) 7_665 3_556
Co2 Al4 Al9 117.67(6) 7_665 3_556
Al1 Al4 Al9 59.48(4) 7_665 3_556
Al2 Al4 Al9 126.76(4) . 3_556
Al3 Al4 Al9 100.62(5) 7_665 3_556
Fe2 Al4 Al9 117.67(6) 7_666 3
Co2 Al4 Al9 117.67(6) 7_666 3
Fe2 Al4 Al9 50.39(3) 7_665 3
Co2 Al4 Al9 50.39(3) 7_665 3
Al1 Al4 Al9 59.48(4) 7_665 3
Al2 Al4 Al9 126.76(4) . 3
Al3 Al4 Al9 100.62(5) 7_665 3
Al9 Al4 Al9 87.42(6) 3_556 3
Fe2 Al4 Ce1 87.78(4) 7_666 1_556
Co2 Al4 Ce1 87.78(4) 7_666 1_556
Fe2 Al4 Ce1 164.03(6) 7_665 1_556
Co2 Al4 Ce1 164.03(6) 7_665 1_556
Al1 Al4 Ce1 123.89(5) 7_665 1_556
Al2 Al4 Ce1 63.84(4) . 1_556
Al3 Al4 Ce1 138.75(3) 7_665 1_556
Al9 Al4 Ce1 64.54(3) 3_556 1_556
Al9 Al4 Ce1 115.91(6) 3 1_556
Fe2 Al4 Ce1 164.03(6) 7_666 .
Co2 Al4 Ce1 164.03(6) 7_666 .
Fe2 Al4 Ce1 87.78(4) 7_665 .
Co2 Al4 Ce1 87.78(4) 7_665 .
Al1 Al4 Ce1 123.89(5) 7_665 .
Al2 Al4 Ce1 63.84(4) . .
Al3 Al4 Ce1 138.75(3) 7_665 .
Al9 Al4 Ce1 115.91(6) 3_556 .
Al9 Al4 Ce1 64.54(3) 3 .
Ce1 Al4 Ce1 77.70(5) 1_556 .
Co2 Al1 Fe2 101.64(7) . 1_556
Co2 Al1 Co2 101.64(7) . 1_556
Fe2 Al1 Co2 0.00(3) 1_556 1_556
Co2 Al1 Al3 57.03(4) . .
Fe2 Al1 Al3 57.03(4) 1_556 .
Co2 Al1 Al3 57.03(4) 1_556 .
Co2 Al1 Al4 57.04(4) . 7_655
Fe2 Al1 Al4 57.04(4) 1_556 7_655
Co2 Al1 Al4 57.04(4) 1_556 7_655
Al3 Al1 Al4 61.08(6) . 7_655
Co2 Al1 Al9 51.42(3) . .
Fe2 Al1 Al9 119.80(6) 1_556 .
Co2 Al1 Al9 119.80(6) 1_556 .
Al3 Al1 Al9 105.13(5) . .
Al4 Al1 Al9 64.28(4) 7_655 .
Co2 Al1 Al9 119.80(6) . 1_556
Fe2 Al1 Al9 51.43(3) 1_556 1_556
Co2 Al1 Al9 51.43(3) 1_556 1_556
Al3 Al1 Al9 105.13(5) . 1_556
Al4 Al1 Al9 64.28(4) 7_655 1_556
Al9 Al1 Al9 92.56(6) . 1_556
Co2 Al1 Al6 119.38(7) . 1_556
Fe2 Al1 Al6 51.50(4) 1_556 1_556
Co2 Al1 Al6 51.50(4) 1_556 1_556
Al3 Al1 Al6 63.93(5) . 1_556
Al4 Al1 Al6 105.07(6) 7_655 1_556
Al9 Al1 Al6 168.25(7) . 1_556
Al9 Al1 Al6 86.63(4) 1_556 1_556
Co2 Al1 Al6 51.50(4) . .
Fe2 Al1 Al6 119.38(7) 1_556 .
Co2 Al1 Al6 119.38(7) 1_556 .
Al3 Al1 Al6 63.93(5) . .
Al4 Al1 Al6 105.07(6) 7_655 .
Al9 Al1 Al6 86.63(4) . .
Al9 Al1 Al6 168.25(7) 1_556 .
Al6 Al1 Al6 91.77(7) 1_556 .
Co2 Al1 Al5 112.09(5) . 3_456
Fe2 Al1 Al5 112.09(5) 1_556 3_456
Co2 Al1 Al5 112.09(5) 1_556 3_456
Al3 Al1 Al5 96.01(7) . 3_456
Al4 Al1 Al5 157.09(8) 7_655 3_456
Al9 Al1 Al5 127.53(4) . 3_456
Al9 Al1 Al5 127.53(4) 1_556 3_456
Al6 Al1 Al5 60.60(4) 1_556 3_456
Al6 Al1 Al5 60.60(4) . 3_456
Co2 Al1 Ce1 89.31(4) . 3_455
Fe2 Al1 Ce1 169.03(5) 1_556 3_455
Co2 Al1 Ce1 169.03(5) 1_556 3_455
Al3 Al1 Ce1 131.77(4) . 3_455
Al4 Al1 Ce1 131.00(4) 7_655 3_455
Al9 Al1 Ce1 66.86(3) . 3_455
Al9 Al1 Ce1 122.24(6) 1_556 3_455
Al6 Al1 Ce1 123.16(6) 1_556 3_455
Al6 Al1 Ce1 68.08(4) . 3_455
Al5 Al1 Ce1 63.32(4) 3_456 3_455
Co2 Al7 Fe1 146.45(8) . 7_655
Co2 Al7 Co1 146.45(8) . 7_655
Fe1 Al7 Co1 0.00(3) 7_655 7_655
Co2 Al7 Co1 146.06(8) . 3
Fe1 Al7 Co1 67.49(5) 7_655 3
Co1 Al7 Co1 67.49(5) 7_655 3
Co2 Al7 Fe1 146.06(8) . 3
Fe1 Al7 Fe1 67.49(5) 7_655 3
Co1 Al7 Fe1 67.49(5) 7_655 3
Co1 Al7 Fe1 0.00(3) 3 3
Co2 Al7 Al8 136.39(3) . 3_556
Fe1 Al7 Al8 52.98(3) 7_655 3_556
Co1 Al7 Al8 52.98(3) 7_655 3_556
Co1 Al7 Al8 52.99(3) 3 3_556
Fe1 Al7 Al8 52.99(3) 3 3_556
Co2 Al7 Al8 136.39(3) . 3
Fe1 Al7 Al8 52.98(3) 7_655 3
Co1 Al7 Al8 52.98(3) 7_655 3
Co1 Al7 Al8 52.99(3) 3 3
Fe1 Al7 Al8 52.99(3) 3 3
Al8 Al7 Al8 87.23(5) 3_556 3
Co1 Al6 Co2 177.91(8) . .
Co1 Al6 Al1 119.12(5) . .
Co2 Al6 Al1 59.71(4) . .
Co1 Al6 Al1 119.12(5) . 1_554
Co2 Al6 Al1 59.71(4) . 1_554
Al1 Al6 Al1 91.77(7) . 1_554
Co1 Al6 Al2 59.13(4) . 1_554
Co2 Al6 Al2 122.02(5) . 1_554
Al1 Al6 Al2 178.08(7) . 1_554
Al1 Al6 Al2 88.60(5) 1_554 1_554
Co1 Al6 Al2 59.13(4) . .
Co2 Al6 Al2 122.02(5) . .
Al1 Al6 Al2 88.60(5) . .
Al1 Al6 Al2 178.08(7) 1_554 .
Al2 Al6 Al2 90.96(7) 1_554 .
Co1 Al6 Al5 58.46(4) . 3_455
Co2 Al6 Al5 120.35(5) . 3_455
Al1 Al6 Al5 121.43(7) . 3_455
Al1 Al6 Al5 60.66(5) 1_554 3_455
Al2 Al6 Al5 57.22(5) 1_554 3_455
Al2 Al6 Al5 117.59(7) . 3_455
Co1 Al6 Al5 58.46(4) . 3_456
Co2 Al6 Al5 120.35(5) . 3_456
Al1 Al6 Al5 60.66(5) . 3_456
Al1 Al6 Al5 121.43(7) 1_554 3_456
Al2 Al6 Al5 117.59(7) 1_554 3_456
Al2 Al6 Al5 57.22(5) . 3_456
Al5 Al6 Al5 89.56(7) 3_455 3_456
Co1 Al6 Al3 125.01(5) . 1_554
Co2 Al6 Al3 56.12(4) . 1_554
Al1 Al6 Al3 115.83(7) . 1_554
Al1 Al6 Al3 56.06(5) 1_554 1_554
Al2 Al6 Al3 65.90(5) 1_554 1_554
Al2 Al6 Al3 125.37(7) . 1_554
Al5 Al6 Al3 91.29(5) 3_455 1_554
Al5 Al6 Al3 176.16(7) 3_456 1_554
Co1 Al6 Al3 125.01(5) . .
Co2 Al6 Al3 56.12(4) . .
Al1 Al6 Al3 56.06(5) . .
Al1 Al6 Al3 115.83(7) 1_554 .
Al2 Al6 Al3 125.37(7) 1_554 .
Al2 Al6 Al3 65.90(5) . .
Al5 Al6 Al3 176.16(7) 3_455 .
Al5 Al6 Al3 91.29(5) 3_456 .
Al3 Al6 Al3 87.63(7) 1_554 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce1 Al1 3.1430(15) 3_556
Ce1 Al1 3.1430(15) 3
Ce1 Al2 3.1521(15) .
Ce1 Al2 3.1521(15) 1_554
Ce1 Al5 3.1605(15) .
Ce1 Al5 3.1605(15) 1_554
Ce1 Al3 3.1937(15) 1_554
Ce1 Al3 3.1937(15) .
Ce1 Al6 3.2048(16) .
Ce1 Al4 3.2116(15) 1_554
Ce1 Al4 3.2117(15) .
Ce1 Al9 3.2808(5) 3
Co2 Al9 2.3430(7) .
Co2 Al6 2.3554(17) .
Co2 Al7 2.4620(17) .
Co2 Al3 2.5248(14) .
Co2 Al3 2.5248(14) 1_554
Co2 Al4 2.5267(15) 7_654
Co2 Al4 2.5267(15) 7_655
Co2 Al1 2.5987(15) 1_554
Co2 Al1 2.5988(15) .
Co1 Al6 2.3359(17) .
Co1 Al8 2.4604(11) .
Co1 Al8 2.4604(11) 1_554
Co1 Al7 2.5430(18) 7_665
Co1 Al7 2.5427(17) 3_455
Co1 Al5 2.5782(14) 3_455
Co1 Al5 2.5782(14) 3_456
Co1 Al2 2.5819(14) 1_554
Co1 Al2 2.5819(14) .
Co1 Co1 2.8253(15) 5_565
Co1 Fe1 2.8253(15) 5_565
Al8 Fe1 2.4604(11) 5_566
Al8 Co1 2.4604(11) 5_566
Al8 Fe1 2.4604(11) 5_565
Al8 Fe1 2.4604(11) 1_556
Al8 Co1 2.4604(11) 1_556
Al8 Co1 2.4604(11) 5_565
Al8 Al2 2.6473(16) .
Al8 Al2 2.6473(16) 5_566
Al8 Al5 2.6564(16) 7_665
Al8 Al5 2.6564(16) 3_456
Al9 Fe2 2.3430(7) 5
Al9 Co2 2.3430(7) 5
Al9 Al1 2.7874(14) 5
Al9 Al1 2.7874(14) 5_556
Al9 Al1 2.7874(14) 1_554
Al9 Al1 2.7874(14) .
Al9 Al4 2.9152(14) 3_455
Al9 Al4 2.9152(14) 7_655
Al9 Al4 2.9152(14) 3_456
Al9 Al4 2.9152(14) 7_654
Al2 Fe1 2.5819(14) 1_556
Al2 Co1 2.5819(14) 1_556
Al2 Al4 2.691(2) .
Al2 Al5 2.723(2) 3_456
Al2 Al6 2.8253(18) .
Al2 Al6 2.8253(18) 1_556
Al2 Ce1 3.1521(15) 1_556
Al5 Fe1 2.5782(14) 3
Al5 Co1 2.5782(14) 3
Al5 Fe1 2.5782(14) 3_556
Al5 Co1 2.5782(14) 3_556
Al5 Al8 2.6565(16) 3_556
Al5 Al3 2.707(2) .
Al5 Al2 2.723(2) 3_556
Al5 Al6 2.8599(18) 3_556
Al5 Al6 2.8599(18) 3
Al5 Al1 2.861(2) 3_556
Al5 Ce1 3.1605(15) 1_556
Al3 Fe2 2.5247(14) 1_556
Al3 Co2 2.5247(14) 1_556
Al3 Al1 2.687(2) .
Al3 Al4 2.733(2) 7_655
Al3 Al6 2.9098(18) 1_556
Al3 Al6 2.9099(18) .
Al3 Ce1 3.1937(15) 1_556
Al4 Fe2 2.5267(15) 7_666
Al4 Co2 2.5267(15) 7_666
Al4 Fe2 2.5267(15) 7_665
Al4 Co2 2.5267(15) 7_665
Al4 Al1 2.690(2) 7_665
Al4 Al3 2.733(2) 7_665
Al4 Al9 2.9152(14) 3_556
Al4 Al9 2.9152(14) 3
Al4 Ce1 3.2116(15) 1_556
Al1 Fe2 2.5988(15) 1_556
Al1 Co2 2.5988(15) 1_556
Al1 Al4 2.690(2) 7_655
Al1 Al9 2.7874(14) 1_556
Al1 Al6 2.8059(17) 1_556
Al1 Al6 2.8059(17) .
Al1 Al5 2.861(2) 3_456
Al1 Ce1 3.1430(15) 3_455
Al7 Fe1 2.5430(18) 7_655
Al7 Co1 2.5430(18) 7_655
Al7 Co1 2.5426(17) 3
Al7 Fe1 2.5426(17) 3
Al7 Al8 2.9204(14) 3_556
Al7 Al8 2.9204(14) 3
Al6 Al1 2.8059(17) 1_554
Al6 Al2 2.8253(18) 1_554
Al6 Al5 2.8599(18) 3_455
Al6 Al5 2.8599(18) 3_456
Al6 Al3 2.9099(18) 1_554
